Journal of Nuclear Materials 266±269 (1999) 222±227 Sputtering of beryllium, tungsten, tungsten oxide and mixed W±C layers by deuterium ions in the near-threshold energy range M.I. Guseva a, A.L. Suvorov b,* , S.N. Korshunov a, N.E. Lazarev b a b Russian Research Centre-Kurchatov Institute, Kurchatov Institute of Atomic Energy, Kurchatov Square 1, 123182 Moscow, Russian Federation Institute of Experimental and Theoretical Physics, B. Theremuchkinskay st. 25, 117259 Moscow, Russian Federation Abstract An experimental method of determination of sputtering yield for current-conducting materials under ion bombardment of light gases in the near-threshold energy range has been developed. Such an information is very important in both the purely scienti®c and applied aspects. This method is based on the use of special regimes of ®eld ion microscopic analysis. The procedure of measuring the sputtering yield includes cleaning of the surface in situ by desorption and evaporation of atoms by the ®eld in order to make atomic-clean and atomic-smooth surface. This method permits to observe single vacancies in the irradiated surface, i.e., directly to count the single sputtered atoms. It has been used for beryllium, technically pure tungsten, tungsten oxide and mixed W±C layer on the tungsten irradiated by deuterium ions. The energy dependence of sputtering yield of those materials by deuterium ions at energies ranging from 10 to 500 eV is investigated. Experimental results for beryllium are in a satisfactory agreement with the calculations of Eckstein et al. Substantial connection between threshold energy of the sputtering and condition of oxidized surface of tungsten has been ascertained. The threshold energy for sputtering of oxidized tungsten surface is equal to 65 eV. The threshold energy for sputtering of mixed W±C layer has almost the same value as for the pure W. Ó 1999 Elsevier Science B.V. All rights reserved. Keywords: Beryllium; Carbon deposition; Low energy deuterium incidence; Sputtering yield 1. Introduction Beryllium, carbon±carbon composites and tungsten are considered at present as candidate-materials for International Thermonuclear Experimental Reactor (ITER). The presence of various materials, as the divertor and the ®rst wall components, will unavoidably result in the formation of mixed layers on the surfaces of plasma facing components. Tungsten is characterized by a high mass number and by a high self-sputtering yield, but also by a high threshold energy for sputtering . However, as a result * Corresponding author. Tel.: +7-095 129 9691; fax: +7-095 127 0573; e-mail: [email protected] of the great chemical anity of tungsten to oxygen its surface is oxidized. As shown in experiments, presence of the oxide ®lm on the surface of tungsten produced under a high partial pressure of residual oxygen (8 ´ 10ÿ5 Torr) in the vacuum chamber causes a considerable (approximately by a factor of 10) reduction in the threshold energy for sputtering of W bombarded with light ions, as a result of reduction in the binding energy of tungsten oxide molecules . But in contrast to tungsten the threshold energy for sputtering of BeO is higher than that of pure beryllium. Under conditions of redeposited materials of an ITER divertor, the surface of tungsten will be covered with a mixed W±C layer. Determination of the sputtering threshold energy of tungsten covered with the mixed W±C and oxide layers is of the principal importance. 0022-3115/99/$ ± see front matter Ó 1999 Elsevier Science B.V. All rights reserved. PII: S 0 0 2 2 - 3 1 1 5 ( 9 8 ) 0 0 8 1 9 - 8 M.I. Guseva et al. / Journal of Nuclear Materials 266±269 (1999) 222±227 It should be noted that the experimental determination of the sputtering threshold energy requires the implementation of extremely sensitive high resolution techniques allowing in situ cleaning of the surface and directly to observe each vacancy produced by the bombarding ions on the surface, i.e., to take each atom removed from surface into account. Among modern experimental means of surface diagnostics, the technique of ®eld ion microscopy was used to study the surface structure of atomic layers, production, behaviour and evolution of defects in a crystalline structure, as has been shown in Refs. [2,3] this technique responds to such requirements for current-conducting materials. In this present work the technique of ®eld ion microscopy was ®rst used for determining the threshold energy for sputtering of pure beryllium and tungsten, tungsten oxide and mixed W±C layers on the tungsten surface, bombarded with deuterium ions, as well as the energy dependence of the sputtering yields by deuterium ions in the near-threshold energy range. 2. Experimental technique The ®eld ion microscope is based on the processes taking place in electric ®elds with a strength of 108 ±1010 V/m. The main element of the ®eld ion microscope is a needle-like sample (cathode) and the anode as a ¯uorescent screen. One can realize the processes of evaporation and desorption in strong electric ®elds, along with an autoionization. In such cases, the surface atoms are removed at any temperatures. The phenomenon of desorption is similar, in principle, to that of evaporation by the ®eld. The dierences between the evaporating ®elds and the desorbing ones are related to a dierent nature of the bond among the particles removed from the surface. Field ion microscopic analysis of samples is being completely optimized and standardized  for the study of tungsten and tungsten-based composite materials. In the present work an attempt was made for the ®rst time to ful®ll the same task for beryllium. The extreme diculty of beryllium samples investigation in a ®eld ion microscope arises from a relatively low melting point (1290°C) of beryllium and the rather low binding energy of beryllium atoms, respectively. Following the original technique described in Ref. , the evaporative ®eld value for beryllium was found to be Fe 28 V/nm. This value is much below the electric ®eld strength value required for helium autoionization (helium is the most appropriate gas for obtaining images in ®eld ion microscope; since for its ionization a ®eld strength of Fi 44 V/nm is required). Due to the fact that for beryllium Fe 6 Fi , microscopic images of beryllium in helium are unstable, though providing atomic resolution in a number of areas. 223 To overcome the above diculty, a technique for obtaining and analysis of desorption images (that is, images in vacuum in the own ions ) was realized in the present work. The appearance of single vacancies on the surfaces of irradiated beryllium samples was registered, primarily, by the high-accuracy measurements of the variation in the images general brightness (measurements of the value of desorption current were taken from a micro-channel plate  placed in front of the ¯uorescent screen of the microscope), and only rarely by direct visual observation. The sputtering yield of tungsten and its compounds was determined by direct count of the number of formed vacancies (see, for example, the ®eld-ion image of the surface of a pure tungsten sample in Fig. 1: single vacancies formed during a single irradiation pulse are marked with arrows). The experiments were performed in the ®eld ion microscope . For samples irradiation the technique of pulsed two-step reversal of high strength polarity was developed and applied. Ionization of the gas, serving simultaneously an image-forming purpose, occurred by the mechanism of electron impact at the moment a short high-voltage pulse of reverse (negative) polarity was fed, and the generation of autoelectrons by the sample took place. The duration of such `ion-generating' high-voltage pulses did not exceed 0.1 ls, at amplitude of 5 kV. Together with the high-voltage pulse, a low-voltage negative pulse was applied to the sample with pulse duration being P 10 ls, while the amplitude corresponding to the preset energy of bombarding ions varied from 10 to 500 V with step of 10 V. Concurrently various check analyses were conducted, which realized various sequences of pulses and their parameters. Fig. 1. The ®eld-ion image of the surface of a pure W sample: single vacancies formed during a single irradiation pulse by D ions are marked with arrows. 224 M.I. Guseva et al. / Journal of Nuclear Materials 266±269 (1999) 222±227 Implementation of cleaning the surface from the adsorbed particles and formed ®lms in the process of measuring the sputtering yield in situ allows to carry out the sputtering measurements from an atomic-pure surface. The procedure of measuring of the sputtering yield includes the following operations. (a) Manufacture of pointed samples and their installation in the ®eld ion microscope capable of ensuring three duties of operation: as a proper ®eld ion microscope, as a desorption ion microscope, and as a ®eld-emission microscope . (b) Evacuation of the microscope with subsequent deuterium ®lling; initially vacuum of 3 ´ 10ÿ9 Torr was reached, after deuterium ®lling the pressure was between 10ÿ6 and 10ÿ5 Torr. (c) Preliminary ®eld-ion and (or) desorption microscopic analysis of an initial surface, its cleaning by evaporation in the ®eld in order to make the atomic-clean and atomic-smooth surface. (d) Ionization of the deuterium gas which serve in the same time as imaging gases. (e) Surface irradiation by D ions, providing the pulsed alternation of the voltage polarity at the sample; the energy of bombarding ions is controlled by a change in the amplitude and duration of a direct pulse. (f) Repeated ®eld-ion and (or) desorption microscopic analysis of the irradiated sample surface in order to identify single vacancies in it, i.e., direct count of the sputtered atoms. (g) Evaluation of sputtering yields corresponding to the given energy of bombarding ions. For the same sample the operations (c)±(g) were repeated many times. The number of `irradiating' voltage pulses was varied from 10 to a few hundred in the cases of low values of the sputtering yields. An important step in the process of sputtering yield evaluation was the determination of irradiation ¯uences. In the present work, the irradiation ¯uence was computed from the formulas derived by the authors in Ref.  (see also Ref. ). The required values for average work function u for Be, W, WO and WC (3.92, 4.54, 5.0 and 3.6 eV, respectively) were taken from Ref. . At the speci®ed irradiation parameters the surface point with the tip average radius Ro 100 nm was exposed to 2.5 ´ 107 impacts of D ions per second, or 250 ions per pulse, which corresponds to a ¯ux density of 2.5 ´ 1017 ions/cm2 s. That means for a sputtering yield Y 10ÿ1 about 25 single vacancies are observed on the entire sample surface viewed through the microscope after one irradiating pulse (the ®eld-ion image of the pointed sample tip surface with Ro 100 nm shows P 105 atoms) and equivalent for Y 10ÿ3 only 1 vacancy over 4 pulses. The needle-point samples of Be were produced by electrochemical etching in concentrated H3 PO4 at 30±50 V dc. In the case of tungsten, electrochemical etching went in 1.5 N solution of NaOH at 5±10 V dc. For producing an oxide layer on the surface of tungsten the samples were heated under the atmosphere up to the temperature of 750°C. The ®lms of a W±C mixture were produced by collection of the products of simultaneous tungsten and graphite sputtering by 20 keV Ar ions on the needle-like and massive samples. The thicknesses of oxidized and mixed layers, their roughness and a chemical composition were determined with the pro®lemeter made by Sloan Instruments and by the Auger electron srectroscopy (AES), in combination with the layer-after-layer etching from masssive samples. Phase composition of the targets was investigated using X-ray analysis of crystalline structure in the sliding beam geometry. 3. Results and discussion 3.1. Threshold energy for sputtering In Table 1 the experimental results of sputtering threshold energies by deuterium and helium ions for the pure Be W, mixed W±C layer and for tungsten oxide are compared with those of the published experimental and theoretical data [1,11]. From Table 1 it follows that the values, Eth , measured by the new method for pure beryllium bombarded with D and He ions are in satisfactory agreement with experiments performed for Be irradiated with D and He ions at 923 K in JET tokamak and also with the calculations of Eckstein et al. . The literature value of the sputtering threshold energy for Be at the room temperature during irradiation is considerably higher. The reason for this high value is probably surface oxidation of the beryllium which leads to higher threshold energy for sputtering due to the higher surface binding energy of oxides. No signi®cant dierences are observed between the values of Eth for W and mixed W±C layer bombarded with D ions. The results for W and W±C layer are in a good agreement with an earlier measurement of threshold energy for sputtering of W and W±C by D ions [11±15]. The threshold energy for sputtering of tungsten oxide by deuterium ions measured by ®eld ion microscopic technique is 65 eV, in contrast to the Eth @ 18 eV in Ref. , where tungsten oxide is produced during irradiation with D ions under background oxygen pressure of 8 ´ 10ÿ5 Torr and the yield is measured by the weight loss method. A low Eth is obtained due to an assumed low surface binding energy (EB 0.3 eV) of the tungsten oxide molecules . In our experiments on the surface of tungsten a stable oxide ®lm, 50 nm thick is M.I. Guseva et al. / Journal of Nuclear Materials 266±269 (1999) 222±227 225 Table 1 The measured threshold energies for sputtering compared to literature values No. Material Ion T(K) Eth (eV) experimental 1 Be D <10 2 Be He 3 4 5 6 W W+C WC Tungsten oxide D D D D 78±373 923 293 293 923 293 78±293 293 65 <10 160 150 produced. An estimate of the surface binding energy from Ref.  gives its value of 1.1 eV. The drastic increasing of sputtering threshold energy by D ions for tungsten oxide layer observed by means of the new technique may also be attributed to the differences of sputtered particles composition between these two methods. The new method identi®es only Wvacancies, i.e., counts only the W sputtered atoms, the weight loss method registrates all sputtered surface atoms, including adsorbed atoms and molecules. 3.2. Energy dependence of sputtering yield for beryllium by D and He ions Fig. 2 shows the measured sputtering yields of beryllium bombarded with deuterium and helium ions at energies from 10 to 200 eV (points). The energy dependences of Be sputtering yields with D and He ions calculated by Eckstein et al.  and averaged experimental data for combinations Be±D and Be±He [15,16] are also given in this graph. The agreement between experimental sputtering yields of beryllium measured by the ®eld ion microscopic technique and computer simulation data  is quite good. While the averaged experimental data from Refs. [15,16] in nearthreshold energy range have lower values in comparison with calculated curves due to the presence of oxide ®lm on the beryllium surface. One should note that the production of vacancies in the energy range under study was observed in the ®rst surface layer only. As a result, in the energy range 10± 200 eV, the sputtering of beryllium atoms takes place from the ®rst monolayer on the surface. Eth (eV) experimental [1,11±14] Eth (eV) theoretical 10 [11,14] 26,2  44,5  13,9 [11,14] 175 ; 178  9,8  30  13,9 [11,14] 201 ; 160  171 ; 150  <18  heating in air, the WO-layer thickness on tungsten is 50 nm. The energy dependence of sputtering yields for tungsten by deuterium ions is given in Fig. 3 (curve 1). In Fig. 3 in addition to our experimental results, also experimental (curve 2) and calculated (curve 3) energy dependence of sputtering yield for combination W±D is presented. The sputtering yields of tungsten, measured by various techniques are rather close to each other, being in a suciently good agreement with a theoretical curve. The energy dependence of the sputtering yields for the redeposited W±C layers and WC  also practically coincides (Fig. 4). 3.3. Energy dependence of sputtering yield for W, WO, W±C by deuterium ions The Auger electron analysis of the mixed W±C layer shows that in the layer, 104 nm thick, W and C are distributed uniformly and the oxygen impurity on the surface does not exceed 9.5 at.%. As a result of tungsten Fig. 2. Energy dependence of sputtering yield of Be with D and He ions at room temperature: (d) this work, Be±D ; (m) this work, Be±He ; (1) calculated data for Be±D ; (2) averaged experimental data for Be±D ; (3) calculated data for Be±He ; (4) averaged experimental data for Be±D . 226 M.I. Guseva et al. / Journal of Nuclear Materials 266±269 (1999) 222±227 Fig. 3. Energy dependence of the sputtering yield of tungsten bombarded with deuterium ions: (1) this work, experimental data (d) for W±D ; (2) experimental data (m) for W±D ; (3) calculated data for W±D . Fig. 5. Energy dependence of the sputtering yield of tungsten oxide (curve 1), (curve 2) ± from  and tungsten (curve 3)  bombarded with deuterium ions: (d) this work, experimental data for tungsten oxide; (m) experimental data for W±D under oxygen pressure of 8 ´ 10ÿ5 Torr ; (+) experimental data for W±D . (curve 2), as well as those for pure tungsten (curve 3), are given. In the energy range <100 eV, the sputtering yields for tungsten irradiated under high pressure of oxygen essentially exceed the corresponding sputtering yields measured by the ®eld ion microscopic technique. At E > 350 eV the sputtering yield values for tungsten oxide measured by weight loss technique (curve 2) approach to the sputtering yields for W (curve 3). It means that, when the sputtering yield rises up to 3 ´ 10ÿ4 at./ ion under experimental conditions , the oxide ®lm on the tungsten surface has been sputtered by D ions. 4. Conclusions Fig. 4. Energy dependence of the sputtering yield of mixed W±C layer on tungsten (1) and WC (2) [11,13] bombarded with deuterium ions: (d) this work, experimental data for mixed W±C layer; (m) experimental data for WC [11,13]. An energy dependence of the sputtering yield of tungsten oxide by deuterium ions (curve 1) is given in Fig. 5. For comparison, on the same graph, the experimental data by Roth et al.  for the tungsten sputtered by D ions under oxygen pressure of 8 ´ 10ÿ5 Torr 1. The advantages of the ®eld ion microscopic technique are: The possibility of cleaning the surface in situ from adsorbed atoms and molecules of residual gases, from oxygen ®lm, etc. The possibility to observe each vacancy produced by the bombarding ions upon the surface, i.e., count each sputtered atom. 2. The drastic increasing of the threshold energy for sputtering of tungsten oxide bombarded with deuterium ions is observed. The sputtering threshold, Eth , measured by new ®eld ion microscopic technique is equal 65 eV. 3. The threshold energies for sputtering of pure beryllium irradiated with deuterium and helium ions at M.I. Guseva et al. / Journal of Nuclear Materials 266±269 (1999) 222±227 room temperature are in satisfactory agreement with the calculations of Eckstein et al., but signi®cantly lower than those values determined by the weight loss method at room temperature. 4. The energy dependences of sputtering yield for pure W and for mixed W±C layer on tungsten bombarded with D ions correspond to the earlier published data for W and WC. 5. The production of vacancies in the energy range under study was only observed in the ®rst surface layer. Acknowledgements This work was supported by the International Atomic Energy Agency. References  J. Roth, J. Bohdansky, W. Ottenberger, Data on low energy light ion sputtering, Max-Planck-Institut f ur Plasmaphysik, Report IPP 9/26, 1979.  A.L. Suvorov, Avtoionnaja microskopija radiacionnich defektov v metallach, M.: Energoizdat, 1982. 227  A.L. Suvorov, Struktura i svoistva poverchnostnich atomnich sloev metallov, M.: Energoatomizdat, 1990.  E.W. Muller, T.T. Tsong, Field Ion Microscopy, Principles and Application, Elsevier, New York, 1969.  A.L. Suvorov et al., Atomn. Energ. 38 (1975) 72.  A.F. Bobkov, A.L. Suvorov, Poverchnost 10 (1983) 67.  J.A. Panitz, Progr. Surf. Sci. 8 (1978) 219.  A.L. Suvorov et al., Prib. Techn. Eksp. 6 (1985) 188.  P.A. Bereznjak, V.V. Slezov, Radiotechn. Elektron. 17 (1972) 354.  V.S. Fomenko, Emissionnie svoistva materialov, Kiev: Naukova dumka, 1981.  W. Eckstein, C. Garcia-Rosales, J. Roth, W. Ottenberger, Sputtering data, Max-Planck-Institut f ur Plasmaphysik, Report IPP 9/82, 1993.  J. Bohdansky, Research Co-ordination Meeting on Plasma-interaction Induced Erosion of Fusion Reactor Materials IAEA, Vienna, 1989.  J. Roth, J. Bohdansky, A.P. Martinelli, Proceedings of First Conference on Ion Beam Modi®cation of Materials, Budapest, Hungary, 1978, pp. 1541±1568.  J. Roth, W. Eckstein, M. Guseva, Fusion Eng. Des. 37 (1997) 465.  J. Roth, J. Bohdansky, R.S. Blewer, W. Ottenberger, J. Nucl. Mater. 85&86 (1979) 1077.  J. Roth, W. Eckstein, J. Bohdansky, J. Nucl. Mater. 165 (1989) 199.
© Copyright 2021 Paperzz